Standard Test Method for Compressive Strength of Cylindrical Concrete Specimens
The compressive strength is determined on a right cylinder. The ratio of height to diameter must be between 1.8 and 2.2.
SIGNIFICANCE AND USE
4.1 Care must be exercised in the interpretation of the significance of compressive strength determinations by this test method since strength is not a fundamental or intrinsic property of concrete made from given materials. Values obtained will depend on the size and shape of the specimen, batching, mixing procedures, the methods of sampling, molding, and fabrication and the age, temperature, and moisture conditions during curing.
4.2 This test method is used to determine compressive strength of cylindrical specimens prepared and cured in accordance with Practices C31/C31M, C192/C192M, C617/C617M, C1176/C1176M, C1231/C1231M, and C1435/C1435M, and Test Methods C42/C42M and C873/C873M.
4.3 The results of this test method are used as a basis for quality control of concrete proportioning, mixing, and placing operations; determination of compliance with specifications; control for evaluating effectiveness of admixtures; and similar uses.
4.4 The individual who tests concrete cylinders for acceptance testing shall meet the concrete laboratory technician requirements of Practice C1077, including an examination requiring performance demonstration that is evaluated by an independent examiner.
1.1 This test method covers determination of compressive strength of cylindrical concrete specimens such as molded cylinders and drilled cores. It is limited to concrete having a density in excess of 800 kg/m3 [50 lb/ft3].
1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The inch-pound units are shown in brackets. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. (Warning—Means should be provided to contain concrete fragments during sudden rupture of specimens. Tendency for sudden rupture increases with increasing concrete strength and it is more likely when the testing machine is relatively flexible. The safety precautions given in the Manual are recommended.)
1.4 The text of this standard references notes which provide explanatory material. These notes shall not be considered as requirements of the standard.
Extracted, with permission, from ASTM C39 Standard Test Method for Compressive Strength of Cylindrical Concrete Specimens, copyright ASTM International, 100 Barr Harbor Drive, West Conshohocken, PA 19428. A copy of the standard may be purchased from ASTM International, phone 610-832-9555, e-mail: email@example.com, website: www.astm.org.
FROM THE BLOG...
Orton's 2019 "Introduction to Refractories" short course is coming up in August. This course is an intensive...
01/18/2019New Laboratory Training Course Announced
LABORATORY TRAINING - THERMAL PROPERTIES OF REFRACTORIES - March 19, 20 & 21, 2019 A Three Day Course...
ADVANCED THERMAL PROPERTIES OF REFRACTORIES - October 29 & 30, 2018 A Two Day Course Sponsored by...